1.
4
Imperfections in the Atomic
and Ionic Arrangements
4–1 Calculate the number of vacancies per cm3 expected in copper at 1080oC (just
below the melting temperature). The activation energy for vacancy formation is
20,000 cal/mol.
Solution: (4 atoms/u.c.)
n = = 8.47 × 1022 atoms/cm3
(3.6151 × 10−8 cm)3
nv = 8.47 × 1022 exp[−20,000/(1.987)(1353)]
= 8.47 × 1022 exp(−7.4393) = 4.97 × 1019 vacancies/cm3
4-2 The fraction of lattice points occupied by vacancies in solid aluminum at 660oC is
10−3. What is the activation energy required to create vacancies in aluminum?
Solution: nv /n = 10−3 = exp[−Q/(1.987)(933)]
ln(10−3) = −6.9078 = −Q/(1.987)(933)
Q = 12,800 cal/mol
4–3 The density of a sample of FCC palladium is 11.98 g/cm3 and its lattice parameter is
3.8902 Å. Calculate (a) the fraction of the lattice points that contain vacancies and
(b) the total number of vacancies in a cubic centimeter of Pd.
Solution: (x)(106.4 g/mol)
(a) 11.98 g/cm3 = −8
(3.8902 × 10 cm)3(6.02 × 1023 atoms/mol)
x = 3.9905
4.0 − 3.9905
fraction = = 0.002375
4
35
2.
36 The Science and Engineering of Materials Instructor’s Solution Manual
(b) number = 0.0095 vacancies/u.c. = 1.61 × 1020 vacancies/cm3
(3.8902 × 10−8 cm)3
4–4 The density of a sample of HCP beryllium is 1.844 g/cm3 and the lattice parameters
are ao = 0.22858 nm and co = 0.35842 nm. Calculate (a) the fraction of the
lattice points that contain vacancies and (b) the total number of vacancies in a
cubic cen- timeter.
Solution: Vu.c. = (0.22858 nm)2(0.35842 nm)cos30 = 0.01622 nm3
= 1.622 × 10−23 cm3
(a) From the density equation:
(x)(9.01 g/mol)
1.844 g/cm3 = x = 1.9984
−23
(1.622 × 10 cm3)(6.02 × 1023 atoms/mol)
2 − 1.9984
fraction = = 0.0008
2
0.0016 vacancies/uc
(b) number = = 0.986 × 1020 vacancies/cm3
1.622 × 10−23 cm3
4–5 BCC lithium has a lattice parameter of 3.5089 × 10−8 cm and contains one vacancy
per 200 unit cells. Calculate (a) the number of vacancies per cubic centimeter and
(b) the density of Li.
Solution: 1 vacancy
(a) = 1.157 × 1020 vacancies/cm3
(200)(3.5089 × 10−8 cm)3
(b) In 200 unit cells, there are 399 Li atoms. The atoms/cell are 399/200:
(399/200)(6.94 g/mol)
r= = 0.532 g/cm3
−8
(3.5089 × 10 cm) (6.02 × 10
3 23
atoms/mol)
4–6 FCC lead has a lattice parameter of 0.4949 nm and contains one vacancy per 500 Pb
atoms. Calculate (a) the density and (b) the number of vacancies per gram of Pb.
Solution: (a) The number of atoms/cell = (499/500)(4 sites/cell)
(499/500)(4)(207.19 g/mol)
r= = 11.335 g/cm3
−8
(4.949 × 10 cm) (6.02 × 10
3 23
atoms/mol)
(b) The 500 Pb atoms occupy 500 / 4 = 125 unit cells:
1 vacancy
× [(1/11.335 g/cm3)] = 5.82 × 1018 vacancies/g
125 cells
(4.949 × 10 −8 cm)3
4–7 A niobium alloy is produced by introducing tungsten substitutional atoms in the
BCC structure; eventually an alloy is produced that has a lattice parameter of
0.32554 nm and a density of 11.95 g/cm3. Calculate the fraction of the atoms in the
alloy that are tungsten.
Solution:
11.95 g/cm3 =
3.
CHAPTER 4 Imperfections in the Atomic and Ionic Arrangements 37
(xW)(183.85 g/mol) + (2 − xW)(92.91 g/mol)
(3.2554 × 10−8 cm)3(6.02 × 1023 atoms/mol)
248.186 = 183.85xW + 185.82 − 92.91xW
90.94xW = 62.366 or xW = 0.69 W atoms/cell
4.
There are 2 atoms per cell in BCC metals. Thus:
fw = 0.69/2 = 0.345
4–8 Tin atoms are introduced into a FCC copper crystal, producing an alloy with a lat-
tice parameter of 3.7589 × 10−8 cm and a density of 8.772 g/cm3. Calculate the
atomic percentage of tin present in the alloy.
Solution: (xSn)(118.69 g/mol) + (4 − xSn)(63.54 g/mol)
8.772 g/cm3 =
(3.7589 × 10−8 cm)3(6.02 × 1023 atoms/mol)
280.5 = 55.15xSn + 254.16 or xSn = 0.478 Sn atoms/cell
There are 4 atoms per cell in FCC metals; therefore the at% Sn is:
(0.478/4) = 11.95%
4–9 We replace 7.5 atomic percent of the chromium atoms in its BCC crystal with tanta-
lum. X-ray diffraction shows that the lattice parameter is 0.29158 nm. Calculate the
density of the alloy.
Solution: (2)(0.925)(51.996 g/mol) + 2(0.075)(180.95 g/mol)
r= = 8.265 g/cm3
(2.9158 × 10−8 cm)3(6.02 × 1023 atoms/mol)
4–10 Suppose we introduce one carbon atom for every 100 iron atoms in an interstitial
position in BCC iron, giving a lattice parameter of 0.2867 nm. For the Fe-C alloy,
find (a) the density and (b) the packing factor.
Solution: There is one carbon atom per 100 iron atoms, or 1 C /50 unit cells, or
1/50 C per unit cell:
(a) (2)(55.847 g/mol) + (1/50)(12 g/mol)
r= = 7.89 g/cm3
(2.867 × 10−8 cm)3(6.02 × 1023 atoms/mol)
(b) 2(4π/3)(1.241)3 + (1/50)(4π/3)(0.77)3
Packing Factor = = 0.681
(2.867)3
4–11 The density of BCC iron is 7.882 g/cm3 and the lattice parameter is 0.2866 nm
when hydrogen atoms are introduced at interstitial positions. Calculate (a) the
atomic fraction of hydrogen atoms and (b) the number of unit cells required on aver-
age to contain one hydrogen atom.
Solution: 2(55.847 g/mol) + x(1.00797 g/mol)
(a) 7.882 g/cm3 =
(2.866 × 10−8 cm)3(6.02 × 1023 atoms/mol)
x = 0.0081 H atoms/cell
The total atoms per cell include 2 Fe atoms and 0.0081 H atoms.
Thus:
0.0081
fH = = 0.004
2.0081
(b) Since there is 0.0081 H/cell, then the number of cells containing H
atoms is:
cells = 1/0.0081 = 123.5 or 1 H in 123.5 cells
5.
4–12 Suppose one Schottky defect is present in every tenth unit cell of MgO. MgO has
the sodium chloride crystal structure and a lattice parameter of 0.396 nm. Calculate
(a) the number of anion vacancies per cm3 and (b) the density of the ceramic.
Solution: In 10 unit cells, we expect 40 Mg + 40 O ions, but due to the defect:
40 Mg − 1 = 39
40 O − 1 = 39
(a) 1 vacancy/(10 cells)(3.96 × 10−8 cm)3 = 1.61 × 1021 vacancies/cm3
(b) (39/40)(4)(24.312 g/mol) + (39/40)(4)(16 g/mol)
r= = 4.205 g/cm3
(3.96 × 10−8 cm)3(6.02 × 1023 atoms/mol)
4–13 ZnS has the zinc blende structure. If the density is 3.02 g/cm3 and the lattice param-
eter is 0.59583 nm, determine the number of Schottky defects (a) per unit cell and
(b) per cubic centimeter.
Solution: Let x be the number of each type of ion in the unit cell. There
normally are 4 of each type.
x(65.38 g/mol) + x(32.064 g/mol)
(a) 3.02 g/cm3 = x = 3.9465
(5.9583 × 10−8 cm)3(6.02 × 1023 ions/mol)
4 − 3.9465 = 0.0535 defects/u.c.
(b) # of unit cells/cm3 = 1/(5.9683 × 10−8 cm)3 = 4.704 × 1021
Schottky defects per cm3 = (4.704 × 1021)(0.0535) = 2.517 × 1020
4–14 Suppose we introduce the following point defects. What other changes in each
structure might be necessary to maintain a charge balance? Explain.
(a) Mg2+ ions substitute for yttrium atoms in Y2 O3
(b) Fe3+ ions substitute for magnesium ions in MgO
(c) Li1+ ions substitute for magnesium ions in MgO
(d) Fe2+ ions replace sodium ions in NaCl
Solution: (a) Remove 2 Y3+ and add 3 Mg2+ − create cation
interstitial. (b) Remove 3 Mg2+ and add 2 Fe3+ − create cation
vacancy. (c) Remove 1 Mg2+ and add 2 Li+ − create cation
interstitial.
+
(d) Remove 2 Na and add 1 Fe 2+
− create cation vacancy.
4–22 What are the Miller indices of the slip directions
(a) on the (111) plane in an FCC unit cell
(b) on the (011) plane in a BCC unit cell?
– – – – –
Solution: [0 11], [01 1] [1 11], [ 11 1]
– – – – –
[ 110], [1 10] [ 11 1], [11 1]
– –
[ 101], [10
1]
z z
y y
7.
4–23 What are the Miller indices of the slip planes in FCC unit cells that include the
[101] slip direction?
– – – – – –
Solution: (11 1), ( 11 1) (1 11), (11 1 )
z z
y y
x
x
4–24 What are the Miller indices of the {110} slip planes in BCC unit cells that include
the [111] slip direction?
– – – – – –
Solution: (1 10), ( 110) (0 11), (01 1) (10 1), ( 101)
z z
z
y y y
x x x
4–25 Calculate the length of the Burgers vector in the following materials:
(a) BCC niobium (b) FCC silver (c) diamond cubic silicon
Solution: (a) The repeat distance, or Burgers vector, is half the body diagonal,
or:
b = repeat distance = (1⁄2) ( 3 ) (3.294 Å) = 2.853 Å
(b) The repeat distance, or Burgers vector, is half of the face diagonal,
or:
b = (1⁄2) ( 2a ) = (1⁄2) ( 2 ) (4.0862 Å) = 2.889 Å
o
(c) The slip direction is [110], where the repeat distance is half of the
face diagonal:
b = (1⁄2) ( 2 ) (5.4307 Å) = 3.840 Å
4–26 Determine the interplanar spacing and the length of the Burgers vector for slip on
the expected slip systems in FCC aluminum. Repeat, assuming that the slip system
–
is a (110) plane and a [11 1] direction. What is the ratio between the shear stresses
required for slip for the two systems? Assume that k = 2 in Equation 4-2.
Solution: (a) For (111)/[110],
b = (1⁄2) ( 2 ) (4.04958 Å) = 2.863 Å 4.04958Å
d111 = = 2.338 Å
1+1+1
(b) If (110)/[111], then:
8.
4.04958Å
b= 3 (4.04958 Å) = 7.014 Å d110 = = 2.863 Å
12 + 12 + 0 2
9.
(c) If we assume that k = 2 in Equation 4-2, then
2.338 2.863
(d/b)a = = 0.8166 (d/b)b = = 0.408
2.863 7.014
ta exp(−2(0.8166))
∴ = = 0.44
tb exp(−2(0.408))
4–27 Determine the interplanar spacing and the length of the Burgers vector for slip on
–
the (110)/[1 11] slip system in BCC tantalum. Repeat, assuming that the slip system
–
is a (111)/[1 10] system. What is the ratio between the shear stresses required for
slip for the two systems? Assume that k = 2 in Equation 4-2.
–
Solution: (a) For (110)/[1 11]:
3.3026 Å
b = (1⁄2) ( 3 ) (3.3026 Å) = 2.860 Å d110 = = 2.335 Å
12 + 12 + 0 2
–
(b) If (111)/[1 10],
then: 3.3026 Å
b= 2 (3.3026 Å) = 4.671 Å d111 = = 1.907 Å
12 + 12 +
12
(c) If we assume that k = 2 in Equation 4-2, then:
2.335 1.907
(d/b)a = = 0.8166 (d/b)b = = 0.408
2.86 4.671
ta exp(−2(0.8166))
= = 0.44
tb exp(−2(0.408))
4–37 How many grams of aluminum, with a dislocation density of 1010 cm/cm3, are
required to give a total dislocation length that would stretch from New York City to
Los Angeles (3000 miles)?
Solution: (3000 mi)(5280 ft/mi)(12 in./ft)(2.54 cm/in.) = 4.828 × 108 cm
(4.828 × 108 cm)(2.699 g/cm3)
= 0.13 g
(1010 cm/cm3)
4–38 The distance from Earth to the Moon is 240,000 miles. If this were the total length
of dislocation in a cubic centimeter of material, what would be the dislocation
density?
Solution: (240,000 mi)(5280 ft/mi)(12 in./ft)(2.54 cm/in.) = 3.86 × 1010 cm/cm3
4-41 Suppose you would like to introduce an interstitial or large substitutional atom into
the crystal near a dislocation. Would the atom fit more easily above or below the
dislocation line shown in Figure 4-8(b)? Explain.
Solution: The atom would fit more easily into the area just below the dislocation
due to the atoms being pulled apart; this allows more space into which
the atom can fit.
4–42 Compare the c/a ratios for the following HCP metals, determine the likely slip
processes in each, and estimate the approximate critical resolved shear stress.
Explain. (See data in Appendix A)
10.
(a) zinc (b) magnesium (c) titanium
(d) zirconium (e) rhenium (f) beryllium
Solution: We expect metals with c/a > 1.633 to have a low tcrss: